dynamic force measurement techniques in split hopkinson pressure
DYNAMIC FORCE MEASUREMENT
TECHNIQUES IN SPLIT HOPKINSON PRESSURE
BAR TESTING OF LOW ACOUSTIC IMPEDANCE
MATERIALS USED AS ARMOR INTERLAYER
A Thesis Submitted to
the Graduate School of Engineering and Sciences of
Ġzmir Institute of Technology
in Partial Fulfillment of the Requirements for the Degree of
MASTER OF SCIENCE
in Mechanical Engineering
Ali Kıvanç TURAN
We approve the thesis of Ali Kıvanç TURAN
Examining Committee Members:
Assoc. Prof. Dr. Alper TAġDEMĠRCĠ
Department of Mechanical Engineering
İzmir Institute of Technology
Assoc. Prof. Dr. Bülent Murat ĠÇTEN
Department of Mechanical Engineering
Dokuz Eylül University
Assist. Prof. Dr. Engin ÖZÇĠVĠCĠ
Department of Mechanical Engineering
İzmir Institute of Technology
05 July 2012
Assoc. Prof. Dr. Alper TAġDEMĠRCĠ
Supervisor, Department of Mechanical
İzmir Institute of Technology
Prof. Dr. Mustafa GÜDEN
Co-Supervisor, Department of
İzmir Institute of Technology
Prof. Dr. Metin TANOĞLU
Head of the Department of
Prof. Dr. R. Tuğrul SENGER
Dean of the Graduate School of
Engineering and Sciences
First and foremost, I would like to express my deepest gratitude to my
supervisor, Associate Prof. Dr. Alper TAŞDEMİRCİ, for his mental support and
guidance through this study with his supportive behavior. His approach to overcome the
problems encountered has encouraged me to fulfill this study. I also would like to thank
to my co-advisor Prof. Dr. Mustafa GÜDEN with his valued support throughout the
study. I would like to thank İ. Kutlay ODACI, Ali KARA and Cenk KILIÇASLAN for
their physical and mental support throughout the study as brothers rather than
colleagues. I also would like to thank to Umut SAVACI, Doğuş ZEREN and Yiğit
ATTİLA for their motivational behaviors.
This study, as the ones before, is dedicated to my beloved family. Firstly, I
would thank to my father who has been and will be my idol, Yavuz Selim TURAN, for
his absolute guidance through my entire life. I gratefully thank to my mother, Hülya
TURAN, for raising me with her tender heart. Her innovative vision and aims in life
enhanced my point of view in every aspect. I also would like to thank to my elder
brother, O. Onur TURAN, for being caring and supportive in every nerve wracking
situation with his admirable sense of humor.
Finally, I would like to thank my girlfriend Selin SARI for her patience and
DYNAMIC FORCE MEASUREMENT TECHNIQUES IN SPLIT
HOPKINSON PRESSURE BAR TESTING OF LOW ACOUSTIC
IMPEDANCE MATERIALS USED AS ARMOR INTERLAYER
GoreTM PolarchipTM heat insulating Teflon and Dow ChemicalsTM Voracor CS
Polyurethane were characterized in this study by conducting compression tests at
various strain rates. Quasi-static compression tests were done with a Shimadzu AG-X
conventional test machine while two different modified Split Hopkinson Pressure Bar
(SHPB) systems were used for dynamic compression tests. Since dynamic testing of
soft materials with classical SHPB is problematic due to low signal levels and relatively
higher signal to noise ratio, impact end of transmitter bar was modified with insertion of
piezoelectric force transducers through the SHPB tests of Teflon, thus enabling the
direct measurement of force on specimen. High strain tests of Polyurethane involved
oscillations in both incident and transmitter bar signals. To overcome this, EPDM
rubber pulse shaper was used through the SHPB tests of Polyurethane. Experimental
results were used in numerical study as material model parameters and SHPB tests of
both materials were simulated in LS-DYNA. Experimental study concluded strong
strain rate dependency in both Teflon and Polyurethane, depicting an increase in
maximum stress with the increase in strain rate. Numerical study showed a good
correlation with experiments in terms of bar stresses and damage behavior of
specimens, offering a solution to more complex problems that can be encountered in
ZIRH ARA YÜZEY MALZEMESİ OLARAK KULLANILAN DÜŞÜK
AKUSTİK EMPEDANSLI MALZEMELERİN SPLİT HOPKİNSON
BASINÇ BARI TESTİNDEKİ DİNAMİK KUVVET ÖLÇÜM
Bu çalışmada GoreTM PolarchipTM Teflon ve Dow ChemicalsTM Voracor CS
Poliüretan değişen deformasyon hızlarında basma testi yapılarak karakterize edilmiştir.
Yarı-statik basma testleri için Shimadzu AG-X konvansiyonel test cihazı kullanılırken
dinamik basma testleri için iki adet Split Hopkinson Basınç Barı (SHBB) sistemi
kullanılmıştır. Yumuşak malzemelerin SHBB testlerinde düşük sinyaller ve göreceli
olarak yüksek sinyal/gürültü oranları gözlendiği için, Teflon‟un dinamik testlerinde
ileten çubuğun numune tarafına piezoelektrik kuvvetölçerler eklenmiş ve bu sayede
direkt olarak kuvvet ölçümü yapılmıştır. Poliüretanın yüksek hızlı deformasyon
testlerinde çubuklardan alınan sinyallerde osilasyon görülmüştür. Bu durumun
önlenmesi için Poliüretanın SHBB testlerinde EPDM kauçuktan sinyal şekillendiriciler
kullanılmıştır. Deneylerden elde edilen sonuçlar nümerik çalışmada malzeme modeli
parametreleri olarak kullanılmış ve bu malzemelerin SHBB testleri LS-DYNA‟da taklit
edilmiştir. Deneysel çalışma iki malzemede de güçlü bir deformasyon hızı etkisi
olduğunu göstermiş, deformasyon hızının artması ile maksimum gerilmenin arttığını
göstermiştir. Nümerik çalışma ise çubuk gerilmeleri ve numunelerin hasar alması
bakımından deneysel çalışma ile uyumluluk göstermiş, gelecekte yapılacak daha
karmaşık çalışmalarda bir çözüm sunmuştur.
TABLE OF CONTENTS
LIST OF FIGURES ....................................................................................................... viii
LIST OF TABLES ............................................................................................................ x
CHAPTER 1. INTRODUCTION ..................................................................................... 1
1.1. Introduction ............................................................................................ 1
CHAPTER 2. FUNDAMENTALS OF SPLIT HOPKINSON PRESSURE BAR
TESTING OF LOW ACOUSTIC IMPEDANCE MATERIALS ............. 8
2.1. Introduction ............................................................................................ 8
2.2. Objective and Method .......................................................................... 11
CHAPTER 3. MATERIALS AND EXPERIMENTS .................................................... 15
3.1. Introduction .......................................................................................... 15
3.2. Materials .............................................................................................. 15
3.2.1. GoreTM PolarchipTM Heat Insulating Teflon .................................. 15
3.2.2. Dow ChemicalsTM Voracor CS Polyurethane ................................ 16
3.3. Experiments ......................................................................................... 17
3.3.1. Quasi-Static Tests .......................................................................... 17
3.3.2. High Strain Rate Tests ................................................................... 19
CHAPTER 4. FINITE ELEMENT MODELING........................................................... 24
4.1. Model Description ............................................................................... 24
CHAPTER 5. RESULTS ................................................................................................ 28
5.1. Results of Experimental Study ............................................................ 28
5.1.1. Quasi – Static Test Results ............................................................ 28
5.1.2. Dynamic Test Results .................................................................... 30
5.2. Results of Numerical Study ................................................................. 34
CHAPTER 6. DISCUSSIONS ....................................................................................... 37
CHAPTER 7. CONCLUSIONS ..................................................................................... 48
REFERENCES ............................................................................................................... 50
LIST OF FIGURES
Figure 2.1. Schematic of classical Split Hopkinson Pressure Bar. ................................... 8
Figure 2.2. Effect of striker bar velocity on the loading pulse. ...................................... 10
Figure 3.1. Core-drilled Teflon specimen before experiment. ....................................... 16
Figure 3.2. Core-drilled Polyurethane specimen before experiment. ............................. 17
Figure 3.3. Shimadzu AG-X test machine used through the quasi-static tests. .............. 18
Figure 3.4. Experimental data of Teflon recorded with Steel SHPB. ............................. 19
Figure 3.5. Quartz crystal before bonding. ..................................................................... 20
Figure 3.6. Schematic of modified SHPB used in dynamic testing of Teflon. ............... 21
Figure 3.7. Schematic of pulse shaper implemented SHPB ........................................... 21
Figure 3.8. Pulse shaper ready for experiment. .............................................................. 22
Figure 3.9. Comparison of a standard compression wave and pulse shaper used .......... 23
compression wave. ....................................................................................... 23
Figure 4.1. Finite element model of Teflon. ................................................................... 25
Figure 4.2. Finite element model of Polyurethane. ......................................................... 25
Figure 5.1. Quasi-static test results of Teflon. ................................................................ 29
Figure 5.2. Quasi-static test results of Polyurethane. ..................................................... 30
Figure 5.3. Experimental data recorded from modified SHPB. ...................................... 31
Figure 5.4. Stress-strain graph of Teflon at the average strain rate of 7200 s-1. ............. 32
Figure 5.5. Stress-strain graph of Teflon at the average strain rate of 9500 s-1. ............. 32
Figure 5.6. Experimental data recorded during the dynamic testing of Polyurethane. ... 33
Figure 5.7. Stress-strain graph of Polyurethane at high strain rates. .............................. 34
Figure 5.8. Comparison of experimental and numerical bar responses of Teflon. ......... 35
Figure 5.9. Comparison of experimental and numerical bar responses of
Polyurethane. ............................................................................................... 36
Figure 6.1. Comparison of experimental results of Teflon at various strain rates. ......... 38
Figure 6.2. Comparison of experimental results of Polyurethane at various
strain rates. ................................................................................................... 39
Figure 6.3. Comparison of experimental and numerical force levels on
transmitter bar. ............................................................................................. 40
Figure 6.4. Force histories of front-end and back-end in Polyurethane sample. ............ 41
Figure 6.5. Dimensionless numerical R parameter-strain graph of Teflon. ................... 42
Figure 6.6. Dimensionless R parameter-strain graph of Polyurethane. .......................... 43
Figure 6.7. Comparison of damage behaviors of Teflon a) experiment, ........................ 44
b) numerical model. ..................................................................................... 44
Figure 6.8. A Teflon specimen before and after an SHPB test. ...................................... 45
Figure 6.9. Comparison of damage behaviors of Polyurethane a) experiment,.............. 46
b) numerical model. ..................................................................................... 46
Figure 6.10. A Polyurethane specimen before and after an SHPB test. ......................... 47
LIST OF TABLES
Table 4.1. Material properties of Teflon and Polyurethane used in numerical study. .... 27
Table 4.2. Material properties of bar materials used in numerical study. ....................... 27
Since late 19th century, gun-fired projectiles have become a massive threat to
mankind in war and peace times. Invention of antiaircraft guns, antitank rifles, portable
and submachine guns have brought out the necessity of using protective equipment to
reduce the number of casualties. In this manner, first defensive systems to increase
protection against projectile threat included steel monolithic layers and increasing the
thickness of steel was the main idea to increase safety [1-3]. However, development of
newer weapons such as antitank missiles, shaped charges and hardened long rod
penetrators have resulted in the defeat of conventional armor designs. In search of better
protection, more efficient armor systems and protective equipment have been developed
to lessen the damage initiated to crew and vehicle itself, increasing survivability against
varying threats. For this purpose, ceramic front layer was included to the monolithic
steel armor, aiming to erode the penetrator on the first microseconds of impact and
reduce penetration by decreasing the kinetic energy of projectile due to friction on
impact area. Backing plate was selected as either steel or composite to further absorb
the kinetic energy of penetrator [4-6]. In addition to hard ceramic face, insertion of a
low acoustic impedance interlayer also enhances the ballistic performance of
multilayered armor systems. Different types of materials such as rubber, Teflon and
aluminum foam were used as interlayer materials to distribute concentrated stress
caused by impact of projectile and reduce the damage inflicted to backing plate [7-10].
When developing new armor systems, it is essential to use a laboratory oriented
methodology as well as ballistic testing based on the method of trial-error. For this
purpose, stress wave propagation in an interlayer material can be investigated by
conducting Split Hopkinson Pressure Bar (SHPB) tests. SHPB testing may help to
determine the stress wave propagation of either an individual layer  or all layers of
an multilayered armor systems [12-14].
As a result of previous studies, an interlayer between hard ceramic face and
steel/composite backing plate is essential to enhance ballistic performance. Polymeric
foams with their low acoustic impedance allow those materials to lower the magnitude
and rise time of stress wave transmitted as well as their weight advantage improves
performance of areal density when compared to monolithic armors. Their relatively
higher energy absorption capability also makes them a possible candidate to be used as
an armor interlayer material . Some of the recent studies focus on the feasibility of
soft materials to be used in applications where shock or impact loading may occur.
Thus, proper characterization of those materials and understanding the response of
material to variability in loading is essential to have safer designs. Chen et al  have
investigated the mechanical behavior of RTV 630 silicone rubber and Styrofoam at
different strain rates. A conventional hydraulically driven test machine was used for low
strain rates and a SHPB was occupied for high strain rate testing of selected materials.
Classical SHPB was modified with X-cut quartz crystals added to the middle of
transmitted bar, thus enabling the measurement of force directly. Experiments
concluded that RTV630 silicone rubber and Styrofoam were found to be strain rate
sensitive and modified split Hopkinson pressure bar was found to be three orders of
magnitude as sensitive as a conventional SHPB.
Chen et al  have investigated the high strain rate compressive behavior of
polyurethane foam with four different density values. Materials were tested from low to
high strain rates to demonstrate the effect of strain rate. Quasi-static tests were
conducted with a MTS 810 test machine while high strain experiments were completed
with a modified split Hopkinson pressure bar. Modified SHPB had quartz crystals added
to the specimen end of incident and transmitted bars and thin aluminum discs were
bonded to quartz crystals to cover them from the direct impact. Experimental results
indicated that failure stress increased with the increase in strain rate. Foam density was
found to be effective on mechanical properties and it was observed that failure stress is
directly proportional with polyurethane foam density.
Song et al  have studied the compressive response and failure behavior of
epoxy syntactic foam. Tested material was made of epoxy resin and hollow glass
microspheres where epoxy resin was used as binder and hollow glass microsphere was
used as filler. Experimental part of the study was completed at low and high strain rates,
having strain rate range of 10-4 s-1 to 1900 s-1 while a constitutive material model with
damage effects was developed through the modeling part of the study. Experimental
results indicated strain rate hardening on epoxy syntactic foam at the strain rates
between 550 s-1 and 1030 s-1. Beyond these levels of strain rate, foam was softened due
to strain rate induced damage. Material model used in modeling part of the study had
given consistent results with the experiments.
Song et al  have studied the effect of strain rate on the elastic and cell wall
crushing behavior of polystyrene foam. A conventional test machine was used for quasi
static tests while a quartz crystal attached split Hopkinson pressure bar was occupied for
the tests at high strain rates. Pulse shapers made of copper with varying thicknesses
were used to reduce the slope of loading pulse. After the experiments, threshold strain
value is defined for each test where strain rate became constant, thus making the test
valid. It is concluded that elastic modulus and cell collapse of polystyrene foam was
found to be sensitive to the changes in strain rate.
Compressive response of three different polymeric foams; namely as expanded
polystyrene (EPS), high density polyethylene (HDPE) and polyurethane with two
different densities on each have been investigated by Oullet et al . Low strain rate
testing of chosen materials were completed with an Instron conventional testing
machine while a drop weight test machine was occupied for the tests at the strain rates
of 10 s-1 and 100 s-1. A polymeric Split Hopkinson Pressure Bar made of acrylic bars
was used throughout the dynamic testing of polymeric foams. After the experiments, it
was observed that EPS and HDPE indicated a linear region followed by increasing
crush stress plateaus while linear region was followed by a plateau region with negative
slope throughout the testing of polyurethane. All of the chosen polymeric foams have
exhibited strain rate dependency, depicting the increase in failure stress and reduction in
both failure and densification strain levels.
Song et al  have investigated the compressive properties of epoxidized
soybean oil/clay nanocomposites. Low and high strain rate compressive tests of
epoxidized soybean oil/clay nanocomposites with different percentages of nanoclay
additions were conducted with a hydraulically driven test machine and a modified
SHPB. Epoxidized soybean oil was mixed with clay nanocomposites with percentage of
2% and 5% while a group of specimens were intentionally left absolute to be compared
through the experiments. Cylindrical cut specimens were tested with a hydraulically
driven test machine at lower strain rates. A modified Split Hopkinson Pressure Bar with
the addition of quartz crystals was used through the high strain rate testing of
specimens. Material model developed by Song et al (2004) was used to estimate the
stress of target material. Experimental results have marked significant strain rate
sensitivities and strain hardening was observed for all kinds of specimens through the
experiments. One dimensional material model with five independent material constants
was successful to obtain similar results with experiments.
Subhash et al  investigated the response of polymeric structural foams to
compressive loadings at different strain rate levels. Polymeric foams used in this study
had a density ranging from 0.83 g.cm-3 to 1.46 g.cm-3 while the porosity levels changing
from 50.5% to 6.8%. Low strain rate compression tests were conducted with a servohydraulic test machine at the strain rate of 1.5 x 10-3 s-1. A polymeric SHPB system was
occupied for the dynamic testing of polymeric foams with the density lower than 1.0
g.cm-3 while a SHPB with magnesium bars were used to compress the chosen foams
with density higher than 1.0 g.cm-3. Experiments concluded that in the quasi-static
range, selected materials exhibit increased modulus of elasticity and higher ultimate
stress as the bulk density increases. Also, decrease in failure strain and increase in yield
stress were observed under high strain rate loading conditions.
Bryson et al  studied the mechanical behavior of five different polyurethane
softballs under quasi-static (0.03 s-1) and high strain rate (2780 s-1) loading conditions.
Dynamic stiffness and coefficient of restitution were the main parameters on the
selection of softballs. A load frame measuring the load and displacement were used for
the low strain rate tests while high strain rates were completed using a classical
aluminum split Hopkinson pressure bar with dimensions of 12.7 mm in common
diameter and 229 mm, 914 mm, 914 mm on striker, incident and transmitter bars,
respectively. After the experiments, an increase of 20-50 percent was observed in chord
modulus of polyurethane softballs due to strain rate increase. However, finite element
modeling of polyurethane softballs needs extra experimental input rather than stated in
this study to successfully simulate the mechanical behavior on computational
Stress-strain behavior of one polyurea and three different polyurethanes with
different hard segment contents were investigated by Yi et al . Dynamic mechanical
analysis, quasi-static compressive tests and high strain rate tests were conducted on
polyurea and polyurethanes to study the mechanical behavior of chosen materials. TA
Instruments Q800 dynamic mechanical analyzer was used throughout the mechanical
analyses while Instron servo hydraulic test machine and Zwick screw driven test
machine were occupied for quasi-static tests and measurement of bulk modulus. A
conventional aluminum split Hopkinson pressure bar was used for the dynamic
compressive testing of polyurea and polyurethanes. Through the experiments, highly
non-linear stress-strain behavior was observed in all of the tested polymers, depicting
strong hysteresis and strong strain rate dependency. Cyclic softening was observed on
some of the tested materials whereas some of polyurea and polyurethanes were found to
transition from rubbery-like behavior to leathery-like behavior while one of the
polyurethanes inhibited transition from rubbery-like behavior to glassy-like behavior.
Sarva et al  have investigated the stress strain behavior of a representative
polyurea and representative polyurethane under compressive loading conditions at the
strain rates ranging from 10-3 s-1 to 10000 s-1. Low strain rate tests (10-3 s-1-10-1 s-1) were
done with a Zwick screw driven mechanical tester while MTS 810 servo hydraulic test
machine was used for the tests up to the strain rate of 100 s-1. Two different split
Hopkinson pressure bar systems with different bar lengths were used to reach the strain
rates of 100 s-1 to 10000 s-1. Intermediate strain rate SHPB, having the striker, incident
and transmitter bar lengths of 3 m, 11 m and 11 m, was constructed from aluminum to
reduce impedance mismatch with polymeric samples. A SHPB with 7075-T6 bars were
used to deform samples beyond the strain rate of 1000 s-1. After the experiments,
deformation of polyurea was found to change from rubbery (10-3 s-1) to glassy (5000 s-1)
whereas behavior of polyurethane shifts from rubbery to leathery with the increase in
strain rate. A strong strain rate dependency is also observed through the steps of strain
Polyurea with mass density of 1 g.cm-3 and elastic modulus of 100 MPa was
characterized by Shim et al . Experiments were conducted with an Instron hydraulic
universal testing machine, a classical split Hopkinson pressure bar with aluminum and
nylon bars and a modified split Hopkinson pressure bar with hydraulic actuator. Instead
of striker bar in conventional SHPB, modified SHPB system consisted of a hydraulic
piston as the actuator and nylon bars were used as incident and transmitter bars as in
classical split Hopkinson pressure bar system. Strain gages were bonded on both impact
and specimen ends of incident and transmitter bars to successfully neutralize the wave
dispersion in polymeric bars and transmitter bar was also fixed on non-impacted side.
Conventional split Hopkinson pressure bar systems and hydraulic test machine were
occupied to validate the experimental results of modified SHPB system. Experimental
results of this study confirm the known strain rate dependency of polyurea and
measured stress levels correspond well with experiments conducted on conventional
testing equipment. However, it was also concluded that stability of strain rate during the
experiments was not possible due to finite length of input and output bars.
Muscle tissues and body parts of animals are also investigated to duplicate the
impact behavior of human flesh, aiming to understand the mechanical behavior and
increase the safety under dynamic loading conditions. Song et al  investigated
compressive response of porcine muscle under various strain rates using a conventional
testing machine and a modified SHPB. Since the target material is rather soft and
experimental data is hard to distinguish, classical 7075-T6 aluminum SHPB was
modified with the addition of semi-conductor foil strain gages on transmitted bar.
Quartz crystals were added to the specimen end of both incident and transmitted bars to
monitor force equilibrium at the front and back-end of specimen. Pulse shaper was also
used to control the shape of loading pulse. Since the specimen is very soft and failure
stress of specimen is few Megapascals, inertia effects may overshadow the material
properties. To cancel out inertia effects, specimen geometry was changed from solid to
annular disc. Experiments revealed that in both along and perpendicular to muscle fiber
direction, strain-rate dependent behavior was observed.
Luo et al  have investigated Young‟s modulus of human tympanic
membrane at high strain rates. A modified Split Hopkinson Tension Bar was used
through the high strain rate experiments with the addition of an X-cut quartz crystal disk
mounted on the incident bar, aiming to measure applied force. 7075-T6 aluminum
incident bar and 6061-T6 aluminum hollow transmitted bar was used through the
experiments. Strain rate of 2000 s-1 was reached through the experiments and it can be
interpreted from results that Young‟s modulus of human tympanic membrane shows an
increase with the increase in strain rate. A strong strain-rate dependency is also
observed, indicating the increase of failure stress with the strain rate.
Pervin et al  have investigated the response of bovine liver tissue under
compressive loading. Experimental determination of strain rate effect on the
compressive stress-strain behavior of bovine liver tissue was aimed in this study, with
the strain rates changing from 10-2 s-1 to 3000 s-1. A conventional hydraulically driven
test machine was used for quasi-static and intermediate strain rates while high strain rate
experiments were done with a Split Hopkinson Pressure Bar. A hollow transmission bar
was used to acquire weak signals through the experiments using semi-conductor gages.
Front and back face forces on the specimen were recorded via quartz crystals to ensure
dynamic equilibrium. Ring-shaped specimens were tested at high strain rates to
eliminate inertia effects. Experimental results show that bovine liver tissue indicates
strong strain rate dependency under compressive loading, especially through the high
strain rate region, regardless of the specimen direction along or perpendicular to liver
Saraf et al  studied the dynamic response of soft human tissues using Kolsky
bar technique, aiming to determine bulk modulus and shear stress of various organs in
human body. Specimens were collected from heart, liver, lung and stomach of postmortem human subjects whose causes of death did not affect the organs targeted for this
study. Determination of bulk modulus was done with using an aluminum split
Hopkinson pressure bar with common diameter of 12.7 mm and a confinement tube
with outer diameter of 25 mm. Shear stress values of chosen materials were obtained
using a shear fixture described with details in stated study. Experiments concluded that
behavior of these tissues under dynamic confined compression can be represented by an
approximately linear relationship between volumetric strain and pressure, indicating as
the stomach being the stiffest tissue whereas the lung as the least stiff. In dynamic
shearing, the behavior of these tissues is not linear elastic. Shear stress-strain curves for
depicted tissues exhibit a toe region followed by a rapid growth of the shear stress with
the moderate increases in shear strain.
FUNDAMENTALS OF SPLIT HOPKINSON PRESSURE
BAR TESTING OF LOW ACOUSTIC IMPEDANCE
For the dynamic mechanical characterization of materials used in armor systems,
SHPB testing is inevitable since the mechanical behavior changes abruptly with the
strain rate. As the case investigated in this study, mechanical behavior of polymers were
highly rate sensitive and previous similar studies showed the same characteristics,
higher failure stresses with reduced failure strain values as the strain rate increases.
Split Hopkinson Pressure Bar, originally developed by Kolsky, is a commonly
used tool to test various materials at dynamic loading conditions and also used in this
thesis through the experimental study. Schematic of classical Split Hopkinson Pressure
Bar setup is given in Figure 2.1.
Figure 2.1. Schematic of classical Split Hopkinson Pressure Bar.
Basically, SHPB consisted of a gas gun, striker bar, incident bar, transmitted bar
and the specimen sandwiched between incident and transmitted bars. In this setup, gas
gun is pressurized up to a predetermined pressure. As the pressurized gas is released
from gas gun, striker bar is set into motion and an initial velocity is attained. Once the
striker bar hits to the incident bar face, a stress wave is created at the impacted end of
incident bar, then this wave travels down the incident bar from striker bar end to
incident bar/specimen interface, called “incident wave (inc.)”. When stress wave
reaches the incident bar/specimen interface, part of the stress wave is transferred to
specimen and caused a rapid deformation while part of stress wave is reflected back to
incident bar, called “reflected wave (ref.)”. As the plastic deformation occurs, stress
wave travels in specimen down to transmitter bar/specimen end. At this point, part of
the stress wave is again reflected in specimen while remaining part is transferred to
transmitter bar, called “transmitter wave (trans.)”. Loading duration of stress wave, T,
produced in a SHPB experiment is directly proportional with the length of striker bar
and defined in Equation 2.1,
Where, L is the striker bar length and Cst is the elastic wave speed of the striker bar
material and defined as in Equation 2.2,
Where, E is the elasticity modulus of striker bar and ρ is the mass density of striker bar
material. Velocity of striker bar is controlled with the pressure level in gas gun and
magnitude of stress wave created is directly proportional with striker bar velocity.
Effect of striker bar velocity on the magnitude of stress wave is given in Figure 2.2.
Figure 2.2. Effect of striker bar velocity on the loading pulse.
As the stress wave propagates through the bars, incident, reflected and
transmitted waves are recorded with the strain gages bonded to the surfaces of bars, as
given in Figure 2.1. Due to the high strength of bar materials, the applied stresses
remain in the elastic deformation region, so the stress and strain values of the specimen
can be measured by acquired strains as a function of time from the full bridge strain
gages. Strain and stress of specimen are calculated with the following equations,
Where; εs is the specimen strain, Cb is wave speed of bar material, Ls is the initial length
of specimen, εr is the strain history of reflected wave, Eb is the Young‟s modulus of bar
material, εt is the strain history of transmitter bar, Ab and As are the bar and specimen
Equations given above are only valid if there is force equilibrium in front and
back faces of specimen. State of force equilibrium is checked with dimensionless R
parameter defined in Equation 2.5,
Where F1 and F2 are defined as front and back forces measured on the specimen. Extent
of deviation of stress is defined by R parameter and when the R reaches 0, stress
equilibrium is reached in specimen.
2.2. Objective and Method
Previous studies showed that low acoustic impedance materials used in armor
systems successfully reduced the transmitted stress values and caused significant
amount of time delay. For a typical ballistic impact event, when the projectile hits the
target, layers of armor are compressed as the course of penetration. In order to have
better ballistic protection, this intrinsic low acoustic impedance characteristic must be
kept at higher strain levels. In this study, two different low acoustic impedance
materials, Teflon and Polyurethane, were mechanically characterized at both quasistatic and high strain rates and the potential applicability of both materials as interlayer
material in multilayered armor systems was investigated.
Quasi-static tests serve to understand the behavior of materials at low strain rates
whereas Split Hopkinson Pressure Bar experiments represent dynamic loading
conditions as well as propagation of stress wave in a single layered material. As
described above, during an SHPB experiment, specimen is deformed with rapid
compression of incident bar due to compressive stress wave created with the impact of
striker to incident bar. Due to theory of dynamic testing with SHPB, bars are considered
to remain on elastic region. In order to satisfy this condition, metals with high yield
strength is generally used as bar material and this result in a difference in terms of
density and acoustic impedance during the testing of soft materials. As the one
dimensional stress wave propagates in bar and specimen on Z-axis only, both materials
can be defined as medium with own characteristics hence term of acoustic impedance is
defined in Equation 2.6 as,
where Z0, ρ and c are defined as acoustic impedance, density of medium and wave
speed, respectively. Using Equations 2.2 and 2.6, ratio of acoustic impedances of Teflon
and CPM Rex 76 steel were calculated as 490.78. As expected, preliminary SHPB tests
of Teflon with CPM Rex 76 bars were found to be problematic since it is hard to
distinguish experimental data from the electrical noise in transmitter bar signals. After
the preliminary testing of Teflon, it was thought to be necessary to change or modify the
classical Split Hopkinson Pressure Bar. For this purpose, there are three different routes
available to overcome this problem: i) changing bar material with polymers such as
acrylic to reduce impedance mismatch, ii) using hollow transmitter bar to reduce density
and wave speed to reduce acoustic impedance of transmitter bar and iii) modifying the
classical split Hopkinson pressure bar by adding piezoelectric transducers to directly
measure the force at the specimen/bar interfaces.
Previously, Zhao et al  investigated usage of low impedance polymeric bars
to reduce impedance mismatch. When polymeric bars are used, a sufficiently large
diameter of both specimen and bar is necessary for two reasons: small diameter
specimen may not represent the behavior of material and dynamic buckling may occur
in polymeric bars with small diameter during the test. However, dispersion correction
must be applied to neutralize wave dispersion effects in bars and striker length must be
reduced to eliminate time extension of the incident wave. Wang et al  also focused
on using polymeric bars and generalization of Split Hopkinson Pressure Bar technique
to use viscoelastic bars. Based on Zhu-Wang-Tang viscoelastic constitutive equations
, authors of the study developed an experimentally confirmed generalized method
for usage of polymeric bars. However, dispersion and dissipation behavior of wave
propagation in polymeric bars must be taken into account to avoid erroneous results.
An alternative method for testing soft materials was proposed by Chen et al 
to overcome the problems encountered using viscoelastic bars. 7075-T651 high strength
aluminum was used as bar material in striker and incident bars while hollow transmitter
bar was used to reduce acoustic impedance mismatch between soft specimens and
transmitter bar. After the experiments conducted with RTV 630 silicon, it was
concluded that using hollow bar enabled the termination of physical effects of
viscoelastic bars. However, this method had just improved the amplitude of transmitter
wave by an order of magnitude but did not affect the amplitude of noise. Furthermore, if
chosen material to be tested has very low strength and acoustic impedance, more
reliable experimental technique with higher sensitivity in transmitter bar signal must be
developed to characterize such materials at high strain rates.
In addition to methods of polymeric and hollow bar usage, insertion of quartz
crystals either to the middle of transmitter bar  or specimen ends of both incident
and transmitter bars [16-18, 20, 26, 28] were offered to characterize soft materials.
Quartz crystals with acoustic impedance very close to bar material are used in modified
SHPB setups. Thin disks of bar material were also used to protect brittle crystals from
direct impact. Quartz crystals allow direct measurement of force at both ends of
specimen and more accurate noise-free data can be recorded during SHPB experiment.
Moreover, force equilibrium in a SHPB experiment can be verified with the data
acquired from quartz crystals.
When the aforementioned solution methods are considered, the quartz crystal
implementation to SHPB setup was selected in the current study. Two differently
behaving materials, one with low Poisson‟s ratio and the other with high, were
characterized in this study.
The first material characterized is Teflon. Due to its low strength and acoustic
impedance, the strain read-outs from the strain-gage on the transmitter bar surface are
low even at comparable levels with the electrical noise occurring in the signals. Thus,
quartz crystals are used at the specimen/transmitter bar interface in order to directly
measure the force values during SHPB tests. 7075-T6 Aluminum bars were also used
and the acoustic impedance mismatch between bar and specimen was lowered. Details
of quartz crystal insertion to transmitter bar end are given in Chapter 3.
The second material characterized is Polyurethane. Preliminary SHPB testing on
Polyurethane showed that the transmitted bar signals are significantly higher than those
of Teflon. Thus, signals could successfully be captured using the regular strain gages on
the bar surfaces. However, main problems encountered with Polyurethane are
oscillations in transmitted bar signals. In order to overcome this, pulse shaping was
applied. In this method, the loading rate, slope of compressive pulse, is modified by
placing soft materials between striker and incident bars end, called “pulse shapers” [1518, 20, 24, 26, 28]. In this study, rectangular prisms of EPDM rubber were deformed to
change the shape of stress wave propagating in incident bar. Details of pulse shaping are
given in Chapter 3.
Mechanical characterization involves quasi-static and high strain rate
experiments. During Split Hopkinson Pressure Bar tests, real time deformation of
samples was recorded with a high speed camera at 10800 fps and 22500 fps.
Outputs of experimental study, both experimental data and high speed camera
recordings, were the main sources of input for the numerical study. Strain gage readouts in a typical experiment include voltage history, allowing the measurement of strain
and stress of specimen as well as those of bars, impact velocity of striker bar and
average strain rate. Finite element model of SHPB uses some of the experimental data
such as stress-strain curve as input and if well-defined, numerical model of split
Hopkinson pressure bar can successfully predict additional parameters such as stress
and displacement of each node, internal energies and force levels on bar interfaces, all
of which can be acquired as function of time. Details of numerical study are given in
MATERIALS AND EXPERIMENTS
Characterization of Teflon and Polyurethane were done with experiments
conducted at various strain rates. Experimental study has begun with preparation of
specimen from both materials. Specimens then were compression tested at both quasistatic and high strain rates using Shimadzu AG-I conventional test machine and Split
Hopkinson Pressure Bar, respectively.
3.2.1. GoreTM PolarchipTM Heat Insulating Teflon
The first material to be characterized was GoreTM PolarchipTM heat insulating
Teflon. This material consisted of expanded polytetraflouroethylene (ePTFE) and boron
nitride (BN) is ideal for the applications of filling gaps where large or variable gaps
occur due to irregular surfaces. Ability of good formability and softness was gained
with matrix material ePTFE while additions of BN particles increase thermal
In this study, Teflon was received in sheet form from the manufacturer.
Cylindrical Teflon specimens were cut with a core-drill, having a common thickness of
2.00 mm and diameter ranging from 12.00 mm to 17.40 mm. A Teflon specimen core –
drilled with a bench type drill before an experiment is given in Figure 3.1.
Figure 3.1. Core-drilled Teflon specimen before experiment.
3.2.2. Dow ChemicalsTM Voracor CS Polyurethane
The second material investigated in this study was Dow ChemicalsTM Voracor
CS Polyurethane. Originally developed for thermal insulation in buildings, this material
can also be sprayed on various surfaces for water isolation. Voracor CS Polyurethane
consists of Voracor CS 1344 Polyol and Voracor CS 1293 Isocynate while the polyol
also consist of HCFC 141b blowing agent to make the form of polymeric foam. During
the application on a surface, components of Polyurethane are mixed and sprayed on
target surfaces using high pressure pumps.
In this study, Polyurethane was received in sheets with varying thicknesses. At
the first stage of specimen preparation, Polyurethane was surface grinded to insure
parallel faces. Surface grinded Polyurethane sheet was then core drilled with a bench
type drill and cylindrical specimens were obtained with dimensions of 2.80 mm in
thickness and 14.50 mm in diameter. Polyurethane sheet, core-drill and specimen before
test are given in Figure 3.2.
Figure 3.2. Core-drilled Polyurethane specimen before experiment.
3.3.1. Quasi-Static Tests
Quasi-static tests were done at the Dynamic Testing and Modeling Laboratory,
IZTECH with both Teflon and Polyurethane to obtain material data under quasi – static
loading conditions. Shimadzu AG-X conventional mechanically driven testing machine
with the capacity of 300 kN was used through the experiments, as given in Figure 3.3.
Figure 3.3. Shimadzu AG-X test machine used through the quasi-static tests.
Strain rate was controlled with the cross head speed. As the cross head speed
increases, strain rate increases and specimen is deformed rapidly. Desired cross head
speed can be determined with the desired strain rate with Equation 3.1,
represents cross head speed, ̇ represents strain rate and
of specimen. Stress – strain curves of polyurethane and Teflon were obtained at the
strain rates of 10-3, 10-2 and 10-1.
3.3.2. High Strain Rate Tests
High strain rate tests were carried out using two different Split Hopkinson
Pressure Bar setups. In addition to quasi-static tests, characterization of Teflon and
Polyurethane was done with implementation of quartz crystals to incident bar and pulse
shaper usage during SHPB testing to overcome the problems encountered on testing of
materials with low acoustic impedance.
Initial testing done on Teflon presented a significant amount of noise in the
signals acquired from the strain gages due to impedance mismatch between specimen
and bar material, given in Figure 3.4. Transmitted bar stress levels are remained low as
compared to those of incident. 7075-T6 aluminum bars were used for this purpose
during the study and also classical Split Hopkinson Pressure Bar was modified with
insertion of quartz crystals.
Figure 3.4. Experimental data of Teflon recorded with Steel SHPB.
The specimen strain was calculated from the reflected wave, the voltage level of
which remained high during the test. Since the voltage level from the transmitter bar
was significantly lower than that of incident, a quartz crystal was added to the
specimen/transmitter bar end to allow direct force measurement and improve accuracy
of stress measurement. In this study, Boston Piezo-Optics X-cut quartz crystals with
thickness of 0.254 ± 0.01 mm in same diameter with bars and had a mechanical
impedance very similar to that of bar material (bar: 14.19 x 106 kg.m-1.s-2 quartz crystal:
15.11 x 106 kg.m-1.s-2 ratio: 1.06) were used. An example of quartz crystal before
bonding is given in Figure 3.5.
Figure 3.5. Quartz crystal before bonding.
During the insertion of quartz crystals; specimen and bar ends were cleaned and
degreased. Then equal amounts of epoxy and hardener of CircuitWorks CW 2400
conductive epoxy were taken and mixed about 3 minutes. Mixture of epoxy and
hardener was smeared on specimen end of transmitter bar and quartz crystal to start
bonding. Marked with a dot, positive pole of quartz crystal was faced to specimen and
covered with a 3 mm thick aluminum platen bonded by conductive epoxy to prevent
damaging during the experiment. Solidification of epoxy was further accelerated and
curing was completed with local heating of cohesion area. When the solidification was
finished, poles of quartz crystals were checked with a multimeter and excessive
conductive epoxy was cleaned off to avoid short circuiting. Both platen and transmitter
bar were drilled about 3 mm for quartz crystal cabling and quartz crystal was connected
to Kistler 5010A charge amplifier. Charge created in quartz crystal due to the applied
loading can be measured in terms of voltage with a piezoelectric constant of -2.3x10-12
C.N-1, output of charge amplifier to LDS Genesis data acquisition system was quartz
crystal voltage as a function of time since measured force was converted into voltage
with constant of 2000 N.V-1. Real time deformation of Teflon during SHPB experiments
were also recorded with Photron FastCam high speed camera. Schematic of modified
SHPB set-up for dynamic testing of Teflon is given in Figure 3.6.
Figure 3.6. Schematic of modified SHPB used in dynamic testing of Teflon.
During the SHPB tests of Polyurethane pulse shaper were used to change the
slope and shape of loading pulse by placing an easily deforming material between
striker and incident bars. Schematic of a pulse shaper implemented SHPB setup is given
in Figure 3.7.
Figure 3.7. Schematic of pulse shaper implemented SHPB.
In this study, EPDM rubber was used as pulse shaper. As received EPDM
rubber was in sheet form with the dimensions of 1200 mm, 300 mm, 3 mm in length,
width and thickness, respectively. Final form of the pulse shaper has the dimensions of
1.5 mm, 1.5 mm, 2 mm in length, width and thickness, respectively. Dimensions of
pulse shaper were changed according to velocity of striker bar. A pulse shaper ready for
experiment is given in Figure 3.8.
Figure 3.8. Pulse shaper ready for experiment.
The effect of pulse shaper on the loading pulse can be seen in Figure 3.9. A
regular loading pulse in Split Hopkinson Pressure Bar is in trapezoidal shape with a
steep slope, while this shape of loading pulse is converted to concave upwards profile
with a relatively lower slope when pulse shaper is used, enabling a smoother loading of
Figure 3.9. Comparison of a standard compression wave and pulse shaper used
FINITE ELEMENT MODELING
4.1. Model Description
Split Hopkinson Pressure Bar tests were modeled to study the stress wave
propagation and dynamic deformation of the materials. Commercially available finite
element software LS-DYNA was used through the numerical studies. Meshes of Split
Hopkinson Pressure Bar and specimens were generated using LS-INGRID. Fully
symmetric numerical model of SHPB was prepared using eight-node solid elements.
Experimental and numerical bar responses are compared and close agreement of results
are checked to verify the finite element model. As discussed in Chapter 2, velocity of
striker bar and strains of bars as a function of time can be measured with strain gages in
an actual SHPB experiment. When verified with good correlation of bar responses to
experiment, finite element model of SHPB can give the output of displacement of
nodes, strains and stresses of elements, force levels on bar interfaces, global and
material energies as well.
Finite element model of Split Hopkinson Pressure Bar contained three
components in contact; specimen, incident and transmitter bars. All of the components
were modeled with the dimensions of experimental set-up. In this study, input pulse
propagating through the incident bar was determined in two methods; either defining an
experimentally determined pressure pulse onto the incident bar face or explicitly
modeling striker bar and assigning an initial velocity to it. Former method was used in
modeling of Teflon and latter for Polyurethane since pulse shaping was used. Mesh
biasing is applied in modeling of both Teflon and Polyurethane to refine the meshes in
interfaces of contact. Mesh sensitivity study was conducted in order to determine the
optimum mesh size. For this purpose, three different mesh sizes were used, average
element size of which was 0.225 mm and the optimum mesh size was determined as 0.2
mm for both Teflon and Polyurethane. Specimens of Teflon and Polyurethane are given
in Figure 4.1 and Figure 4.2, respectively.
Figure 4.1. Finite element model of Teflon.
Figure 4.2. Finite element model of Polyurethane.
The material model 63, *MAT_CRUSHABLE_FOAM, was used during the
numerical modeling of Polyurethane and Teflon. This material model was developed to
represent the behavior of strain rate sensitive crushable foams with optional parameters
such as damping coefficient and tension cut-off stress. Through the implementation,
stress in elements was updated using the Equation 4.1,
is principal stresses, E is modulus of elasticity, ̇ is principal strain rate and
is time interval of solution. Magnitude of principal stresses (i=1, 3) are checked if the
value of yield stress is exceeded and if so, they are scaled back to the yield surface using
For a valid Split Hopkinson pressure bar test, incident and transmitter bars must
*MAT_ELASTIC. This material model was developed for isotropic elastic behavior for
beam, shell and solid elements in LS-DYNA. Contact between specimen and bars were
specimen chosen as „slave‟ while static and dynamic coefficient of friction was selected
as 0.3 and 0.2, respectively. Time step calculation was done with automatic time step
calculation option was used with CONTROL_TIMESTEP. In this option, LS-DYNA
determines step size by looping through the elements and taking the minimum value
over all elements. Determination of time step is given in Equation (4.3),
Where, TSSFAC and N are scale factor for computed time step and total number
of elements, respectively. Time step size roughly corresponds to transition time of a
wave through an element using the shortest characteristic distance. Default value of 0.90
was determined by LS-DYNA and was sufficient enough to duplicate wave
characteristics. Material properties of Teflon, Polyurethane and bar materials are given
in Table 4.1 and 4.2.
Table 4.1. Material properties of Teflon and Polyurethane used in numerical study.
9.65 x 10-3
TSC = 50 MPa
DAMP = 0.05
TSC = 50 MPa
DAMP = 0.3
Table 4.2. Material properties of bar materials used in numerical study.
5.1. Results of Experimental Study
5.1.1. Quasi – Static Test Results
Polyurethane and Teflon were tested at strain rates of 10-3 s-1, 10-2 s-1 and 10-1 s-1
using Shimadzu AG-X universal test machine under compression. Before the
experiments, average strain rate of each test was calculated using Equation 3.1. During
the tests, force and cross-head displacement data were recorded. Video extensometer
was also used to measure the specimen strain. This data is then converted to stress-strain
graphs at each strain rate.
Quasi-static test results of Teflon are given in Figure 5.1. It can be seen from
figure that all of the tests in quasi-static range showed similar characteristics under
quasi-static compressive loadings regardless of strain rate. All three curves started with
a linear region, a plateau region with a slight slope then this region was followed by
densification. Densification strain was found to vary with strain rate. At the average
strain rate of 10-3 s-1, a maximum stress of 15 MPa was reached at a strain of 0.85 while
maximum strain was reduced to 0.77 for the average strain rate of 10-2 s-1. Maximum
strain was further reduced to 0.6 at the average strain rate of 10-1 s-1. Macroscopically,
Teflon was found to fail completely after the experiments and tested specimens were
smeared on both ends of cross-heads.
Figure 5.1. Quasi-static test results of Teflon.
Polyurethane was tested at average strain rates of 10-3 s-1, 10-2 s-1 and 10-1 s-1 and
results are given in Figure 5.2. It can be interpreted from the figure that Polyurethane
shows a linear region up to a strain of 0.1 in all of the quasi-static tests conducted.
Above the strain of 0.1, a plateau region with a slight slope was observed regardless of
strain rate. As strain is increased, a sudden increase in stress of Polyurethane was
observed in quasi-static tests, showing the initiation of densification. At the average
strain rate of 10-3 s-1, maximum stress of 85 MPa was reached at the strain of 0.8 while
maximum stress was increased to 95 MPa at the average strain rate of 10-2 s-1. As the
average strain rate was increased to 10-1 s-1, maximum stress reached on polyurethane
was increased to 100 MPa while peak strain value was reduced to 0.76. On macroscopic
scale, when force was removed, instantaneous elastic recovery was observed with no
Figure 5.2. Quasi-static test results of Polyurethane.
5.1.2. Dynamic Test Results
Dynamic testing of Teflon was carried out using 7075-T6 aluminum Split
Hopkinson Pressure Bar with quartz crystal implemented. Typical data recorded
through a SHPB experiment of Teflon is given in Figure 5.3. Solid and dashed lines in
Figure 5.3 represent the signals measured with strain gages mounted on incident and
transmitter bars, respectively while dotted line represents the recordings of quartz
crystal. During the experiment, initial rise of compressive pulse in transmitter bar was
observed about 275 µs in quartz crystal recordings while strain gage on transmitter bar
has started to obtain signals at 380 µs. The difference between initiation of data
acquisition in quartz crystal and strain gage can be related with the position of those
sensors on transmitter bar. Also, a good correlation was observed in transmitter bar
signals acquired with strain gage and quartz crystal in terms of amplitude and
magnitude of signal.
Figure 5.3. Experimental data recorded from modified SHPB.
As stated in Chapter 2, strain and strain rate of a SHPB test can be altered by
varying the striker bar velocity. During SHPB testing of Teflon, striker velocity of 16.34
m/s and 21.42 m/s were reached, resulting the average strain rates of 7200 s-1 and 9500
s-1 in experiments, respectively. High strain rate test results of Teflon at the average
strain rates of 7200 s-1 and 9500 s-1 were given in Figures 5.4 and 5.5, respectively. It
can be interpreted from aforementioned figures that measurements of stress with strain
gages involved oscillations up to strain of 0.08 and followed by underestimation of
specimen stress up to the strain of 0.15. Above the strain of 0.15, stress-strain curves of
strain gage and quartz crystal tend to follow similar trend. Both of quartz crystal and
strain gage have reached the same level of maximum strain and maximum stress during
SHPB testing. At the average strain rate of 7200 s-1, a maximum stress around 10 MPa
was reached at a strain of 0.3 while maximum stress was increased to 80 MPa at the
average strain rate of 9500 s-1. After SHPB tests, Teflon specimens were failed
completely and smeared to impact end of transmitter bar.
Figure 5.4. Stress-strain graph of Teflon at the average strain rate of 7200 s-1.
Figure 5.5. Stress-strain graph of Teflon at the average strain rate of 9500 s-1.
High strain rate testing of Polyurethane was carried out using steel Split
Hopkinson Pressure Bar. Bar material was selected as VASCOMAX C350 maraging
steel due to material‟s superior mechanical properties and typical experimental data
recorded during the testing of Polyurethane is given in Figure 5.6. It can also be seen
from figure that oscillations in the loading and output pulses were reduced by the
deformation of EPDM rubber pulse shaper between striker and incident bars.
Dimensions of pulse shaper were determined by conducting empty tests (no specimen
between the bars) for various striker bar velocities. When a striker of 700 mm was used,
pulse shaper of EPDM cube with a side dimension of 1.5 mm was used for the SHPB
testing of Polyurethane at lower strain rates. For the tests at higher strain rates, the shape
of pulse shaper was changed to rectangular prism accordingly to dimensions of 1.5 mm
x 1.5 mm x 2 mm.
Figure 5.6. Experimental data recorded during the dynamic testing of Polyurethane.
Dynamic compression stress-strain curves of Polyurethane are given in Figure
5.7. Triangle-marked line in Figure 5.7 represents the lowest strain rate achieved
through the SHPB testing of Polyurethane (1360 s-1) whereas dashed line and solid line
represent the two other results of SHPB tests at the average strain rates of 1650 s-1 and
2260 s-1, respectively. Results indicate that regardless of strain rate, stress-strain
behavior of Polyurethane follow a similar trend of curves with two different slopes on
each. Up to a strain of 0.1, all of the curves represent a linear region with steeper slopes
when compared to quasi-static tests. As the strain of 0.1 was reached, slope of strainstress curve was reduced, again regardless of strain rate. At the average strain rate of
1360 s-1, maximum stress of 42 MPa was reached at a strain of 0.35 while maximum
stress was increased to 56 MPa and 107 MPa at the average strain rates of 1650 s-1 and
2260 s-1, respectively. All three curves indicated unloading after reaching maximum
stress values at the average strain rates. On macroscopic scale, no visible damage or
rupture was also observed on specimens subjected to dynamic compressive loadings.
Figure 5.7. Stress-strain graph of Polyurethane at high strain rates.
5.2. Results of Numerical Study
SHPB experiments conducted with Teflon and Polyurethane were numerically
modeled using LS-DYNA finite element software. Bar response of an SHPB experiment
done with Teflon was compared with numerical study in Figure 5.8. In this figure,
dotted line represents the SHPB experiment of Teflon while solid line represents the
result of numerical study and both curves were shifted in time domain to simplify
distinguishing. As seen from Figure 5.8 that numerical study agreed well with
experiment in terms of amplitude and magnitude of stress waves both in incident and
transmitter bars. It was also concluded that the wave propagation in aluminum SHPB
was well duplicated with numerical model of Teflon and allowed to have detailed
information about “black box” of SHPB testing with additional outputs mentioned in
Figure 5.8. Comparison of experimental and numerical bar responses of Teflon.
Numerical bar response of Polyurethane was compared with an SHPB
experiment in Figure 5.9. Bar response of numerical study on Polyurethane is
represented with dotted line while bar response of experiment conducted with steel
SHPB is represented with solid line. Both of the curves again intentionally shifted in
time domain to simplify distinguishing the results of numerical and experimental
studies. A good correlation was observed between numerical and experimental study in
shape of bar responses both in incident and transmitter bars. Matching of bar responses
also concluded that wave propagation in steel SHPB was well modeled through the
numerical study and allowed having further information on SHPB testing of
Polyurethane, mentioned in Chapter 6.
Figure 5.9. Comparison of experimental and numerical bar responses of Polyurethane.
As stated in previous chapters, experimental study involves testing of Teflon and
Polyurethane at various strain rates. Mechanical properties of both materials were
determined with quasi-static and high strain rate compression tests, reaching the lowest
strain rate of 10-3 s-1 in quasi-static tests while 2260 s-1 and 9500 s-1 in SHPB tests of
Polyurethane and Teflon, respectively.
Through the experimental study, quasi-static tests of Teflon were conducted at
the strain rates of 10-3 s-1, 10-2 s-1 and 10-1 s-1 while strain rate was increased to 7200 s-1
and 9500 s-1 during SHPB tests. Compression stress strain curves of Teflon at various
strain rates are given in Figure 6.1. It can be interpreted from figure that experimental
results of Teflon indicated similar characteristics against compressive loading. For
comparison, maximum stress of 15 MPa was taken as the uppermost level of stress for
quasi-static and SHPB tests. At the strain rate of 10-3 s-1, maximum stress was reached
at a strain around 0.8 while maximum strain was reduced to 0.1 at the strain rate of 9500
s-1 and depicted strong strain rate dependency. Densification strain was also found to be
decreased with the increasing strain rate due to rapid stiffening behavior on Teflon with
the increase in strain rate.
Figure 6.1. Comparison of experimental results of Teflon at various strain rates.
Compressive stress-strain curves of Polyurethane at various strain rates are given
in Figure 6.2. Quasi-static tests were conducted at the strain rates of 10-3 s-1, 10-2 s-1 and
10-1 s-1 whereas strain rates of 1360 s-1, 1650 s-1 and 2260 s-1 were reached at SHPB
tests. Quasi-static compression tests presented a linear region followed by plateau
region with a small slope. Linear region in quasi-static regime nearly ended at the strain
of 0.1 with same slope on each strain rate and modulus of elasticity was found to be
around 46MPa. Between the strain of 0.1 and 0.2, stress-stain curves began to diverge.
Finally, around the strain of 0.8, stress-strain curves can easily be distinguished,
reaching the maximum stresses of 100 MPa, 95 MPa and 85 MPa with the increasing
strain rate, respectively. For high strain rate regime, experimental results of
Polyurethane displayed two linear regions with different slopes. Rapid compression of
specimens in SHPB testing of polyurethane have resulted a sharp rise up to a strain of
0.1. Beyond the strain of 0.1, all of the stress-strain curves had a tendency to increase
with a relatively smaller slope, reaching the final stress values of 42 MPa, 56 MPa and
107 MPa with the increasing strain rate, followed by unloading. In light of these
consequences, experiments concluded strain rate dependency in Polyurethane and rate
dependency is more pronounced with the increased strain levels.
Figure 6.2. Comparison of experimental results of Polyurethane at various strain rates.
Numerical study focused on finite element modeling of SHPB experiments.
Primary motivation is to verify the material model constants and to investigate the wave
propagation inside material and dynamic deformation sequences; if numerical data, bar
response, correspond well with experiment, material model constants can be further
used in application of different impact events such as armor penetration. As stated
before, Figure 5.8 and Figure 5.9 represent the comparison of bar responses and
indicated a good correlation between numerical model and experimental results is noted.
In addition, numerical model can provide additional information such as stress histories
of specimen and force history of bars.
Figure 6.3 shows the comparison of transmitter bar force levels of Teflon both
experimentally and numerically. Dashed line in Figure 6.3 represents experimental
while solid line represents numerical. It can be seen from figure that experimental and
numerical data do not correspond well up to 250 µs due to stress inequilibrium inside
the specimen. This also verifies the necessity of quartz crystal usage during the tests.
After 280 µs, experimental and numerical curves follow similar trend and greater
correlation is observed up to 310 µs, which also shows the stress equilibrium.
Figure 6.3. Comparison of experimental and numerical force levels on transmitter bar.
Comparison of axial force histories of front-end and back-end of specimen is
given in Figure 6.4. Solid line in Figure 6.4 indicates the force history of front-end
while force history of back-end is represented by dotted line. A slight deviation was
observed between those curves during the loading phase while as the deformation
continues, dynamic stress equilibrium was reached. However, front-end and back-end
force histories do not match during unloading. In light of these consequences, it can be
concluded that slight variations occur between front-end and back-end force histories
during loading and unloading.
Figure 6.4. Force histories of front-end and back-end in Polyurethane sample.
Stress equilibrium in Split Hopkinson Pressure Bar experiments can be checked
with dimensionless R parameter defined in Equation 2.5. Figure 6.5 indicates the
variation of numerical R parameter with strain at the strain rate of 7200 s-1. As seen in
Figure 6.4, R converges to zero around strain of 0.4 after which stress equilibrium is
reached in specimen.
Figure 6.5. Dimensionless numerical R parameter-strain graph of Teflon.
Force equilibrium in finite element model of Polyurethane was also investigated
and R parameter-strain graph at 1360 s-1 is given in Figure 6.6. It can be interpreted
from the figure that the value of R converges from 1.5 to 0 about a strain of 0.18,
indicating stress equilibrium is reached.
Figure 6.6. Dimensionless R parameter-strain graph of Polyurethane.
Real time damage behavior of Teflon during a SHPB test at 9500 s-1 was
monitored at 10800 fps and comparison of experimental and numerical deformation
profiles at three different time steps, 0 µs, 92 µs and 184 µs were given in Figure 6.7.
The first row in Figure 6.7 represents the non-deformed specimens in both numerical
and experimental study (0 µs). At 92 µs, while stress wave propagated through incident
bar, specimen was compressed between incident and transmitter bars and expanded
radially. At 184 µs, the last row of Figure 6.7, Teflon was fully compressed and tended
to lose shape completely while being smeared on incident and transmitter bar interfaces.
It can be concluded from the figure that mechanical behavior of Teflon is well
duplicated in numerical model. A Teflon specimen before and after SHPB test is given
in Figure 6.8.
Figure 6.7. Comparison of damage behaviors of Teflon a) experiment,
b) numerical model.
(cont. on next page)
Figure 6.7. (cont.).
Figure 6.8. A Teflon specimen before and after an SHPB test.
Real time deformation behavior of Polyurethane at the strain rate of 1360 s-1 was
recorded using high speed camera at 22500 fps during the SHPB test and recorded
images were compared with those of numerical study in Figure 6.9. The first row of
images represents the non-compressed samples in experimental and numerical studies (0
µs). As the stress wave traveled down the incident bar, specimens were compressed
down to intermediate strain levels (44 µs). At 132 µs, as the strain was increased,
Polyurethane was compressed and expanded radially while the length was reduced. No
visible damage was observed through the experimental and numerical studies.
Comparison of damage in Polyurethane specimen is given in Figure 6.10.
Figure 6.9. Comparison of damage behaviors of Polyurethane a) experiment,
b) numerical model.
(cont. on next page)
Figure 6.9. (cont.).
Figure 6.10. A Polyurethane specimen before and after an SHPB test.
In this study, GoreTM PolarchipTM heat insulating Teflon and Dow ChemicalsTM
Voracor CS Polyurethane were characterized by conducting experiments at both quasistatic and high strain rates. Quasi-static tests were carried out using Shimadzu AG-X
conventional test machine while SHPB set-up was used for high strain rate tests. During
the high strain rate testing of Teflon, a quartz crystal implemented aluminum SHPB was
used in order to minimize the problems associated with acoustic impedance mismatch
between the bars and specimen. For SHPB testing of Polyurethane, steel bars along with
pulse shapers were used. Pulse shaping reduced the oscillations occurring in input and
output bar responses. Real time deformation of Teflon and Polyurethane was also
recorded with a high speed camera.
After mechanical characterization, appropriate material models and their
parameters were determined. SHPB tests were modeled using LS-DYNA 971 and
material model parameters were checked by comparing experimental and numerical
results. For both materials, crushable foam material model was successfully used. This
well verified material can then be further used in the simulation of more complex
impact problems such as armor penetration.
Experimental and numerical study revealed the following conclusions;
Teflon indicated strong strain rate dependency. Quasi-static test results involved
linear, plateau and densification regions, while a linear region followed by
densification in SHPB tests.
Strain rate dependency was also observed for Polyurethane. Quasi-static tests
depicted linear, plateau and densification regions, while SHPB tests indicated
two linear regions with different slopes.
A well verified set of constants for each material was determined. Numerical
results also confirmed the necessity of quartz crystal usage in SHPB testing of
Teflon. Stress equilibrium was reached at low strain levels in SHPB testing of
Polyurethane. Numerical deformation behaviors were also in accordance with
those of experimental.
For the future work, these well verified material model parameters can further be
used in simulating more complex problems such as penetration of armors containing
these interlayers. These simulations can shed into light to the optimization of
multilayered armor systems.
B. R. Sorensen, K. D. Kimsey, G. F. Silsby, D. R. Scheffler, T. M. Sherrick, and
W. S. de Rosset, "High velocity penetration of steel targets," International
Journal of Impact Engineering, vol. 11, pp. 107-119, 1991.
D. L. Littlefield, C. E. Anderson Jr, Y. Partom, and S. J. Bless, "The penetration
of steel targets finite in radial extent," International Journal of Impact
Engineering, vol. 19, pp. 49-62, 1997.
T. Børvik, M. Langseth, O. S. Hopperstad, and K. A. Malo, "Ballistic
penetration of steel plates," International Journal of Impact Engineering, vol.
22, pp. 855-886, 1999.
S. Sadanandan and J. G. Hetherington, "Characterisation of ceramic/steel and
ceramic/aluminium armours subjected to oblique impact," International Journal
of Impact Engineering, vol. 19, pp. 811-819, 1997.
J. López-Puente, A. Arias, R. Zaera, and C. Navarro, "The effect of the thickness
of the adhesive layer on the ballistic limit of ceramic/metal armours. An
experimental and numerical study," International Journal of Impact
Engineering, vol. 32, pp. 321-336, 2005.
B. A. Roeder and C. T. Sun, "Dynamic penetration of alumina/aluminum
laminates: experiments and modeling," International Journal of Impact
Engineering, vol. 25, pp. 169-185, 2001.
B. A. G. Gama, J. W., T. A. Bogetti, H. Mahfuz, and B. Fink, "Effect of nonlinear material behavior on the through-thickness stress wave propagation in
multi-layer hybrid lightweight armor," Adv Comput Eng Sci Technol Sci Press,
pp. 157-62, 2000.
B. A. Gama, T. A. Bogetti, B. K. Fink, C.-J. Yu, T. Dennis Claar, H. H. Eifert,
and J. W. Gillespie Jr, "Aluminum foam integral armor: a new dimension in
armor design," Composite Structures, vol. 52, pp. 381-395, 2001.
B. A. G. Gama, J. W., T. A. Bogetti, and B. Fink, "Innovative design and
ballistic performance of lightweight composite integral armor," presented at the
SAE 2001 World Congress, Detroit, MI, 2001.
A. Tasdemirci, G. Tunusoglu, and M. Güden, "The effect of the interlayer on the
ballistic performance of ceramic/composite armors: Experimental and numerical
study," International Journal of Impact Engineering, vol. 44, pp. 1-9, 2012.
A. Tasdemirci, A. Kara, A. K. Turan, G. Tunusoglu, M. Guden, and I. W. Hall,
"Experimental and Numerical Investigation of High Strain Rate Mechanical
Behavior of a [0/45/90/ - 45] Quadriaxial E-Glass/Polyester Composite,"
Procedia Engineering, vol. 10, pp. 3068-3073, 2011.
A. Tasdemirci and I. W. Hall, "Numerical and experimental studies of damage
generation in multi-layer composite materials at high strain rates," International
Journal of Impact Engineering, vol. 34, pp. 189-204, 2007.
A. Tasdemirci and I. W. Hall, "The effects of plastic deformation on stress wave
propagation in multi-layer materials," International Journal of Impact
Engineering, vol. 34, pp. 1797-1813, 2007.
A. Tasdemirci and I. W. Hall, "Development of novel multilayer materials for
impact applications: A combined numerical and experimental approach,"
Materials & Design, vol. 30, pp. 1533-1541, 2009.
W. Chen, F. Lu, and B. Zhou, "A quartz-crystal-embedded split Hopkinson
pressure bar for soft materials," Experimental Mechanics, vol. 40, pp. 1-6, 2000.
W. Chen, F. Lu, and N. Winfree, "High-strain-rate compressive behavior of a
rigid polyurethane foam with various densities," Experimental Mechanics, vol.
42, pp. 65-73, 2002.
B. Song, W. Chen, and D. J. Frew, "Dynamic Compressive Response and
Failure Behavior of an Epoxy Syntactic Foam," Journal of Composite Materials,
vol. 38, pp. 915-936, 2004.
B. Song, "Strain-rate effects on elastic and early cell-collapse responses of a
polystyrene foam," International Journal of Impact Engineering, vol. 31, pp.
S. Ouellet, D. Cronin, and M. Worswick, "Compressive response of polymeric
foams under quasi-static, medium and high strain rate conditions," Polymer
Testing, vol. 25, pp. 731-743, 2006.
B. Song, W. Chen, Z. Liu, and S. Erhan, "Compressive properties of epoxidized
soybean oil/clay nanocomposites," International Journal of Plasticity, vol. 22,
pp. 1549-1568, 2006.
G. Subhash, Q. Liu, and X. Gao, "Quasistatic and high strain rate uniaxial
compressive response of polymeric structural foams," International Journal of
Impact Engineering, vol. 32, pp. 1113-1126, 2006.
A. Bryson and L. Smith, "Impact response of sports materials," Procedia
Engineering, vol. 2, pp. 2961-2966, 2010.
J. Yi, M. C. Boyce, G. F. Lee, and E. Balizer, "Large deformation ratedependent stress–strain behavior of polyurea and polyurethanes," Polymer, vol.
47, pp. 319-329, 2006.
S. S. Sarva, S. Deschanel, M. C. Boyce, and W. Chen, "Stress–strain behavior of
a polyurea and a polyurethane from low to high strain rates," Polymer, vol. 48,
pp. 2208-2213, 2007.
J. Shim and D. Mohr, "Using split Hopkinson pressure bars to perform large
strain compression tests on polyurea at low, intermediate and high strain rates,"
International Journal of Impact Engineering, vol. 36, pp. 1116-1127, 2009.
B. Song, W. Chen, Y. Ge, and T. Weerasooriya, "Dynamic and quasi-static
compressive response of porcine muscle," J Biomech, vol. 40, pp. 2999-3005,
H. Luo, C. Dai, R. Z. Gan, and H. Lu, "Measurement of young's modulus of
human tympanic membrane at high strain rates," J Biomech Eng, vol. 131, p.
064501, Jun 2009.
F. Pervin, W. W. Chen, and T. Weerasooriya, "Dynamic compressive response
of bovine liver tissues," J Mech Behav Biomed Mater, vol. 4, pp. 76-84, Jan
H. Saraf, K. T. Ramesh, A. M. Lennon, A. C. Merkle, and J. C. Roberts,
"Mechanical properties of soft human tissues under dynamic loading," J
Biomech, vol. 40, pp. 1960-7, 2007.
H. Zhao, G. Gary, and J. R. Klepaczko, "On the use of a viscoelastic split
hopkinson pressure bar," International Journal of Impact Engineering, vol. 19,
pp. 319-330, 1997.
L. Wang, K. Labibes, Z. Azari, and G. Pluvinage, "Generalization of split
Hopkinson bar technique to use viscoelastic bars," International Journal of
Impact Engineering, vol. 15, pp. 669-686, 1994.
W. Chen, B. Zhang, and M. Forrestal, "A split Hopkinson bar technique for lowimpedance materials," Experimental Mechanics, vol. 39, pp. 81-85, 1999.